- Open Access
Assessment of waste clays in the Qusseir region of east central Egypt for production of lightweight bricks
© The Author(s) 2018
- Received: 29 June 2018
- Accepted: 6 September 2018
- Published: 3 October 2018
Egyptian Upper Cretaceous waste clay samples from Yunis Mines, Qusseir vicinity, Eastern Desert, were investigated for their chemical and mineralogical compositions as well as for firing. These investigations were carried out to assess the suitability to use the waste clays for the production of lightweight bricks. X-ray fluorescence (XRF), scanning electron microscopy (SEM), X-ray diffraction (XRD), and Fourier transform infrared (FTIR) techniques were applied for characterizing chemical and mineral compositions of the raw clays. On the other side, densification parameters of the fired samples up to 1100 °C were examined by using Archimedes water-saturation methods and by determining the density and crushing strength of the fired bodies.
Two types of concrete were prepared using different grain sizes: coarse and a mix of coarse and fine aggregates. Concrete batches were prepared, and the mechanical strength and the bulk density were determined. Mineralogically, the waste samples consist of montmorillonite as the predominant clay mineral, with quartz, calcite, fluorapatite, anhydrite, and pyrite as impurities. Bulk density and apparent porosity of the fired clay sample at 1100 °C were 0.89 g/cm3 and 67.19%, respectively, while the bulk density of the two types of concrete range from 0.76 g/cm3 in coarse type with no fines to 0.90 g/cm3 in the coarse with 20% fine fraction. The crushing strength of both types is 25 kg/cm2 for coarse type and 45 kg/cm2 for coarse and fine types, respectively.
The results showed that the data provides a useful application of waste clay ramps of ancient Yunis mining tunnels in Qussier area with an additional mean to assess their suitability for the production of lightweight brick concretes to reduce density and their relatively good strength in modern buildings for non-loading building units and to enhance the thermal insulation of buildings.
Clay deposits are widely distributed within many geological formations from Carboniferous to recent age. They are located in the region of Nile Valley and Delta, as well as in the Western and Eastern Desert of Egypt. Most of these deposits are used for the applications in many ceramic industries, for example, whiteware, refractories, heavy clay products, and Portland cement (Hanna and Stoops 1977; Said 1990; Youssef 2008). Clays are classified according to their particle size, mineral and chemical compositions, and other properties (Grim 1962, 1968; Grimshaw 1971; Norton 1969; Konta 1979, Burst 1991). Many authors indicated that kaolinite-rich clay materials are refractory with a high vitrification range, low plasticity, white-to-buff burning colour and a low-drying and firing shrinkage. Moreover, montmorillonite-rich clays are non-refractory with low vitrification ranges, high plasticity, buff-to-red burning colour, and a high-drying and firing shrinkage. In contrast, illite-rich clays are falling between kaolinitic and montmorillonitic clays and exhibit wide variations. Lightweight clay aggregates may be produced by firing pellets of low-grade montmorillonite-rich clays with or without adding to the vitrification range. After firing, the clay pellets swell or bloat owing to gas releases within the firing bodies during the liquid phase. On cooling, these low-grade montmorillonite clays conserve the cellular texture, and lightweight aggregate is obtained (Serry et al. 1985; Konta 1995; Karaman et al. 2006; Bernhardt et al. 2013; Ismail et al. 2016, Ismail et al. 2018; Risdanareni et al. 2017).
Many authors have studied the effect of using a pore-forming agent to increase the porosity of the ceramic body such as Duchan and Kopar (2001), Chemani and Chemani (2013), and Ismail et al. (2016). Others studied the replacement of cement with lighter materials, e.g. Mashaly et al. (2016, 2018), Bian et al. (2012) and Pelisser et al. (2012). Also, clay and pore-forming agent are shaped insulating refractory bricks with a true porosity of more than 45% and a service temperature of at least 800 °C (Grimshaw 1971; Sargeant and Stone 1981; Courtault et al. 1983; Routschka 1997).
The chemical and mineralogical compositions of these clays were studied using XRF, XRD, FTIR, and SEM techniques. The chemical composition of the studied samples was determined by using an Axios Sequential WD_XRF Spectrometer, PAnalytical 2005 in the National Research Center Laboratories, Dokki, Cairo, Egypt. ASTM E 1621 standard guide for elemental analysis by wavelength-dispersive X-ray fluorescence spectrometer and the ASTM D 7348 standard test method for loss on ignition (LOI) on solid combustion were used as guidelines. X-ray diffraction analysis (XRD) was performed on a Philips X-ray diffractometer, Mod. PW 1390, with Ni-filtered Cu-Kd radiation. The morphology and the microstructure of the samples were characterized with SEM coupled with energy-dispersive spectroscopy EDAX (SEM Model Quanta FEG 250) carried out in the National Research Center Laboratories. FTIR absorption spectra were recorded by Elmer-783 double-beam dispersion spectrophotometer using standard KBr tablets. Three hundred milligram KBr was homogenized with 1 to 2 mg of the sample in a vibration mill and evacuated, and the tablets were then pressed for 5 min under pressure of 10 MPa. The recording time was 20 min, and the range is 4000–400 cm−1.
The preparation of lightweight brick regime starts with the firing of a crushed representative waste clay sample at 1100 °C and then broke up using a jaw crusher until obtaining a grain size ranging from 2 to 10 mm with minimum amounts of finer-grained material. Two mixes of concrete were prepared using two different grain sizes of the fired waste clay grains: the first mix consisted of coarse grains ranged from 2 to 10 mm with no fines, and the second mix composed of coarse grains (2 to 10 mm) with 10% finer ones. The percentages of the cement and water were applied as per standard specification (British standard 2028 1968). The concretes were casted into cubic molds with a dimension of 5 × 5 × 5 cm3 then demolded after 24 h and cured in ~ 95% humidity chamber for 28 days. The prepared cubes were tested for crushing strength and bulk density according to ASTM C20 2010.
Characterization of the waste clays
Chemical analyses of the used sample in weight %
XRD analysis indicated that the main mineral component of the raw waste clays is montmorillonite, with calcite, fluorapatite, gypsum, and quartz impurities. Pyrite was also detected as in the clay-size fraction.
Densification parameter of the fired samples at 1100 °C
Type of the clay
Bulk density (g/cm3)
Apparent porosity (%)
Raw waste clay
Fired waste clay
Properties of the casted mixes
Mix composition and properties of the prepared lightweight concrete
Type of the fired waste clay aggregate in the mixture
Mix composition (ratio by volume)
Bulk density (g/cm3)
Crushing strength (kg/cm2)
Coarse aggregate (2–10 mm grain size)
Coarse aggregate with 10% finer particles
Effect of clay firing
Table 2 indicates that the bulk density of the fired clay decreased from 2.21 g/cm3 for the raw waste clay to 0.89 g/cm3, while the apparent porosity increased from 6.55% for the raw waste clay to 67.19% after firing. The enormous expansion indicated by the porosity is due to the gasses generated by oxidation of the organic material contained in the raw clay, note in Fig. 5 the absence of organic matter bands from the fired sample IR pattern due to the oxidation. This expansion occurs until the surfaces of the particles have attained sufficient strength to prevent the gasses from escaping.
Assessment of lightweight bricks
To consider the blocks produced from the fired aggregates as lightweight bricks according to the British Specification No. 2028, bulk density should be between 0.55 and 1.05 g/cm3. The bulk density of the concretes ranges from 0.76 to 0.90 g/cm3 for the coarse type with no fine aggregates mix 1 and the coarse type with 10% fine aggregates mix 2, respectively (Table 3). The crushing strength of both types after curing for 28 days was 25 kg/cm2 for coarse-grained types only and 45 kg/cm2 for coarse-fine-grained types. The above results indicate that the concretes, containing the fine portion of the grain sizes, gave a higher compressive strength and a higher density than those without any fine fractions. Therefore, it is possible to produce lightweight concrete blocks of low density and relatively good strength to be utilized in modern building trend for non-loading building units and in the partition wall construction, as well as for improving the thermal insulation of buildings.
The materials used in this work were waste clays from Yunis mines, which are located south of the Hamrawin area and 12 km from Qusseir–Safaga Asphaltic Road to the west.
XRF, XRD, FTIR, and SEM data confirmed that the predominant mineral components present are montmorillonite, with quartz, calcite, fluorapatite, gypsum, and pyrite impurities.
Bulk density and apparent porosity of the fired samples at 1100 °C are 0.89 g/cm3and 67.19%, respectively.
Two types of concrete were prepared using two different grain size fractions of the fired waste clay grains. The first grain type ranges from 2 to 10 mm with no fines while the second contains the coarse grows (2 to 10 mm) with a 10% finer fraction.
The bulk density of the two types of concrete ranges between 0.76 g/cm3 in coarse-grained type with no fines and 0.90 g/cm3 in the coarse-grained fraction with 10% fine fraction. The crushing strength of both types after curing for 28 days is 25 kg/cm2 for coarse type and 45 kg/cm2 for coarse and fine types.
The thousands of small, air-filled cavities give the two types their strength and thermal insulation properties. The base material was waste clay and was fired up to 1100 °C. Finally, the clay materials were mixed and molded to form lightweight concrete block products.
The above results indicate the possibility of producing low-density and relatively high-strength concrete block products for the utilization in modern building trend for dead-load construction for partition wall construction, as well as for improving the thermal insulation of buildings.
This study was funded by the NRC project titled “Effect of soil pollution and geochemical characteristics on its productivity and its relation to electrical properties.”
Availability of data and materials
The authors declare that the work data and material are available.
EAE-A, HM, and WA contributed in the field, geochemistry, mineralogy, and application works. ME contributed to the mineralogy, physical parameters, and application works. All authors read and approved the final manuscript.
Ethics approval and consent to participate
The authors declare that the work is ethically approved and consent to participate.
Consent for publication
The authors declare that the work has a consent for publication.
The authors declare that they have no competing interests.
- ASTM C20 (2010) Standard test methods for apparent porosity, water absorption, apparent specific gravity, and bulk density of burned refractory brick and shapes by boiling water. Annual Book of ASTM Standards, ASTM International, West ConshohockenGoogle Scholar
- Bernhardt M et al (2013) Mechanical properties of lightweight aggregates. J Eur Ceram Soc 33:2731–2743View ArticleGoogle Scholar
- Bian Z, Miao X, Lei S, Chen SE, Wang W, Struthers S (2012) The challenges of reusing mining and mineral-processing wastes. Science 337(6095):702–703ADSView ArticleGoogle Scholar
- British standard 2028 (1968) Precast concrete blocks. British Standards Institution BS 2028:1968. BSI, London, EnglandGoogle Scholar
- Burst JF (1991) The application of clay minerals in ceramics. Appl Clay Sci 5(5–6):421–443ADSView ArticleGoogle Scholar
- Chemani H, Chemani B (2013) Valorization of wood sawdust in making porous clay brick. Sci Res Essays 8(15):609–614Google Scholar
- Courtault B, Brand JP, Boisson G (1983) “Carbonaceous shales”, Cim., Betons, plastres, Chaux, vol 39, p 740Google Scholar
- Duchan V, Kopar T (2001) Sawdust and paper-making sludge as pore forming agents for lightweight clay bricks source. Ind Ceram 21(2):81–86Google Scholar
- Gadsden JA (1975) Infrared spectra of minerals and related inorganic compounds. Butterworths, LondonGoogle Scholar
- Grim RE (1962) Applied clay mineralogy. Mc Graw Hill Book Comp., Inc., New York, Toronto, LondonGoogle Scholar
- Grim RE (1968) Clay mineralogy, 2nd edn. Mc Graw Hill Book Comp., Inc., New York, Toronto, LondonGoogle Scholar
- Grimshaw RW (1971) The chemistry and physics of clays and other ceramic materials. Ernst Benn, LondonGoogle Scholar
- Hanna FS, Stoops G (1977) Micromorphological description of some clayey basin irrigated soils [clay, silty clay, Egypt]. Egypt J Soil Sci. 17;1:21–33Google Scholar
- Ismail AIM, Souaya ER, El-Hakeem AA (2016) Assessment of different shapes and grain sizes of bentonite aggregates in lightweight concretes. Interceram-Int Ceramic Rev 65(3):96–99View ArticleGoogle Scholar
- Ismail AIM, Souaya ER, Fathy M, El-Hakeem AA (2018) Production of lightweight concretes from pumice/bentonite mix. Geotech Geol Eng 36(1):581–588View ArticleGoogle Scholar
- Karaman S, Gunal H, Ersahin S (2006) Assesment of clay bricks compressive strength using quantitative values of colour components. Constr Build Mater 20:348–354View ArticleGoogle Scholar
- Keller WD, Reynolds RC, Inoue A (1986) Morphology of clay minerals in the smectite – to – illite conversion series by scanning electron microscopy. Clay Clay Miner 34(2):187–197ADSView ArticleGoogle Scholar
- Konta J (1979) Deposits of ceramic raw materials. Ceramic Monographs-Handbook of Ceramics, Verlag Schmid GmbH, Freiburg, Monograph, 1(3).Google Scholar
- Konta J (1995) Clay and man: clay raw materials in the service of man. Appl Clay Sci 10:275–335View ArticleGoogle Scholar
- Mashaly AO, El-Kaliouby BA, Shalaby BN, El–Gohary AM, Rashwan MA (2016) Effects of marble sludge incorporation on the properties of cement composites and concrete paving blocks. J Clean Prod 112:731–741View ArticleGoogle Scholar
- Mashaly AO, Shalaby BN, Rashwan MA (2018) Performance of mortar and concrete incorporating granite sludge as cement replacement. Constr Build Mater 169:800–818View ArticleGoogle Scholar
- Norton FH (1969) Refractories, 4th edn. Mc Graw Hill Book Comp., Inc., New York, Toronto, LondonGoogle Scholar
- Pelisser F, Barcelos A, Santos D, Peterson M, Bernardin AM (2012) Lightweight concrete production with low Portland cement consumption. J Clean Prod 23(1):68–74View ArticleGoogle Scholar
- Risdanareni P, Choiri AA, Djatmika B, Puspitasari P (2017) Effect of the use of metakaolin artificial lightweight aggregate on the properties of structural lightweight concrete. Civ Eng Dimens 19(2):86–92Google Scholar
- Routschka G (ed) (1997) Refractory materials: pocket manual. Vulkan Verlag EssenGoogle Scholar
- Said R (1990) The geology of Egypt, 2nd edn. A. A. Balkeema Publishers, RotterdamGoogle Scholar
- Sargeant GK, Stone RE (1981) Inventors; Cawoods Refractories Ltd, assignee. Process for manufacturing a lightweight refractory product. United States patent US 4,307,051.Google Scholar
- Serry MA, Hegab M, Elbana MM (1985) Lightweight clay aggregates from Wadi El- Natrun clays (Egypt). Sprechsael 118:N Y11Google Scholar
- Youssef AM (2008) Mapping the Pliocene clay deposits using remote sensing and its impact on the urbanization developments in Egypt: case study, East Sohag area. Geotech Geol Eng 26(5):579–591View ArticleGoogle Scholar